Precisely tunable magnetic phase transition temperature, TC, through the formation of a molecular alloy in [NixPt1-x(mnt)2](-)-based spin systems (mnt(2-) = maleonitriledithiolate, x = 0.09-0.91).
Yuan, Guo-Jun; Yang, Hao; Liu, Shao-Xian; Liu, Jian-Lan; Ren, Xiao-Ming; Dalton transactions (Cambridge, England : 2003) 43 (2014) 11908–11914; doi:10.1039/c4dt00868e

data_7031328
_publ_section_title
;
 Precisely tunable magnetic phase transition temperature, TC, through the
 formation of a molecular alloy in [NixPt1-x(mnt)2](-)-based spin systems
 (mnt(2-) = maleonitriledithiolate, x = 0.09-0.91).
;
_journal_issue                   31
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11908
_journal_page_last               11914
_journal_paper_doi               10.1039/c4dt00868e
_journal_volume                  43
_journal_year                    2014
_chemical_formula_sum            'C20 H11 Cl N5 Ni0.91 Pt0.09 S4'
_chemical_formula_weight         555.35
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 102.627(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.1224(15)
_cell_length_b                   26.281(3)
_cell_length_c                   7.3751(9)
_cell_measurement_temperature    296(2)
_cell_volume                     2292.8(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0516
_diffrn_reflns_av_sigmaI/netI    0.0507
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -34
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            20998
_diffrn_reflns_theta_full        27.61
_diffrn_reflns_theta_max         27.61
_diffrn_reflns_theta_min         2.32
_exptl_absorpt_coefficient_mu    1.794
_exptl_crystal_density_diffrn    1.609
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1117
_refine_diff_density_max         0.409
_refine_diff_density_min         -0.332
_refine_diff_density_rms         0.080
_refine_ls_extinction_coef       0.0034(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     282
_refine_ls_number_reflns         5294
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.019
_refine_ls_R_factor_all          0.0698
_refine_ls_R_factor_gt           0.0408
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0405P)^2^+0.3094P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0891
_refine_ls_wR_factor_ref         0.1011
_reflns_number_gt                3653
_reflns_number_total             5294
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4dt00868e2.cif
_cod_data_source_block           NiPt91
_cod_depositor_comments
'Adding full bibliography for 7031320--7031328.cif.'
_cod_database_code               7031328